**Damage and dissipation mechanisms in the dynamic fracture**

**of brittle materials: Velocity driven transition from nominally**

**brittle to quasi-brittle**

J. Scheibert123,a, C. Guerra14, D. Dalmas2, and D. Bonamy1

1 _{CEA, IRAMIS, SPCSI, Group Complex Systems and Fracture, F-91191 Gif-sur-Yvette, France}
2 _{Unit´e Mixte CNRS/Saint-Gobain, Surface du Verre et Interfaces, 39 Quai Lucien Lefranc, 93303}

Aubervilliers cedex, France

3 _{Physics of Geological Processes, University of Oslo, Oslo, Norway}

4 _{Facultad de Ingenier´ıa Mec´anica y El´ectrica, Universidad Aut´onoma de Nuevo Le´on, Avenida }
Uni-versidad, S/N, Ciudad Universitaria, C.P. 66450, San Nicol´as de los Garza, NL, Mexico

**Abstract.** *We present the results of recent dynamic fracture experiments [Scheibert et*
* al., Phys. Rev. Lett. 104 (2010) 045501] on polymethylmethacrylate, the archetype of*
nominally brittle materials, over a wide range of crack velocities. By combining velocity
measurements and finite element calculations of the stress intensity factor, we determine
the dynamic fracture energy as a function of crack speed. We show that the slope of this
curve exhibits a discontinuity at a well-defined critical velocity, below the one associated
to the onset of micro-branching instability. This transition is associated with the
appear-ance of conics patterns on the fracture surfaces. In many amorphous materials, these are
the signature of damage spreading through the nucleation, growth and coalescence of
micro-cracks. We end with a discussion of the relationship between the energetic and
fractographic measurements. All these results suggest that dynamic fracture at low
ve-locities in amorphous materials is controlled by the brittle/quasi-brittle transition studied
here.

**1 Introduction**

Driven by both technological needs and the challenges of unresolved fundamental questions, dynamic fracture in brittle materials has been widely investigated over the past century. Since the pionneer work of Griffith [1], Orowan[2] and Irwin[3] a coherent theoretical framework, the Linear Elastic Fracture Mechanics (LEFM) has developed. This theory is based on the fact that – in an elastic medium under tensile loading – the mechanical energy released as fracture occurs is entirely dissipated at the crack tip within a small zone so-called process zone. Defining the fracture energyΓas the energy needed to create two crack surfaces of a unit area, the crack growth velocity is then selected by the balance between the energy flux and the dissipation rateΓv. This yields [4]:

Γ_{≃}(1−v/c*R) K*2*(c)/E,* (1)

*where cRand E are the Rayleigh wave speed and the Young modulus of the material, respectively, and*
*K(c) is the Stress Intensity Factor (SIF) for a quasi-static crack of length c. K depends only on the*
applied loading and specimen geometry, and characterizes entirely the stress field in the vicinity of the
crack front.

a _{e-mail:}_{julien.scheibert@fys.uio.no}
© Owned by the authors, published by EDP Sciences, 2010

LEFM provides a quantitative description of crack motion that agrees well with observations as
long as the crack growth is sufficiently slow [5]. However, comparisons between theory and
experi-ments at high speed yield large discrepancies (see [7,6] for recent reviews). In particular, contrary to
what is predicted by LEFM, (i) the maximal crack speeds attained experimentally in amorphous
ma-terials are far slower than the limiting speed*cR*predicted by Eq. (1) and (ii) fracture surfaces become

rough at the optical scale at high velocities (the so-called mirror_{→}mist_{→}hackle transition).
The existence of a micro-branching instability [11,12] at a critical velocityv*b*=0.4*cR*may explain

*part*of this discrepancy: Beyondv*b*, the crack motion stops to be a single crack state to become a

mul-tiple crack state that cannot be described by Eq. 1 anymore. And it has been argued [10] thatv*b*sets the

limit beyond which experiments start to depart from theory. The understanding and modelling of the
micro-branching instability hence yielded many recent theoretical efforts [13–22]. However, a number
of puzzling observations remain at smaller velocities. In particular, even for velocities much lower
thanv*b*, (i) the measured dynamic fracture energy is generally much higher than that at crack initiation

[10,23–26] and (ii) fracture surfaces roughen over length scales much larger than the microstructure scale (”mist” patterns) [27], the origin of which remains debated [28–37].

In this paper, we present recent results [38] of dynamic fracture experiments in
polymethyl-methacrylate (PMMA), the archetype of brittle amorphous materials, designed to unravel the primary
cause of these last discrepancies. We show that the slope of the dynamic fracture energy as a function
of crack speed exhibits a discontinuity at a well-defined critical velocityv*a*well belowv*b*. This

tran-sition coincides with the onset of damage spreading through the nucleation, growth and coalescence of micro-cracks, the signature of which is the presence of conic patterns on post-mortem fracture sur-faces. We provide a simple interpretation for this nominally brittle to quasi-brittle transition allowing to relate both the energetic and fractographic measurements.

**2 Experiments**

0 20 40 60 80

0 50 100 150 200 250 300 350 400

Crack length (mm)

Crack velocity (

m/

s)

0 20 40 60 80

0 0.5 1 1.5 2 2.5 3 3.5 4 4.5

Crack length (mm)

SIF

(M

P

a.m

1/2

)

*c*
*v*

**Fig. 1.**Adapted from [38]. Left: Measured crack velocityvas a function of crack length*c*in a typical

experi-ment (*U*0=2.6 J). The vertical lines are error bars. Right: Calculated quasi-static SIF*K*as a function of*c*. Inset:

Schematics of the Wedge-Splitting test.

Dynamic cracks are driven in PMMA with measured Young modulus and Poisson ratio of*E*=2.8_{±}0.2
GPa andν=0.36, which yields *cR*=880±30 m.s−1. Its fracture energy at the onset of crack

propa-gation was determined to be*K*2

*c*/*E*=0.42±0.07 kJ.m−2, with*Kc*being the material toughness.

Frac-ture tests are performed in a so-called wedge splitting geometry [39]. Parallelipedic specimen of size
140×125×15 mm3 in the *x* (propagation),y(loading) and *z*(sample thickness) are prepared by
cutting out of one of the two 125_{×}15 mm2_{faces a 25}

Two steel jaws equipped with rollers are then placed on both sides of the mouth and a steel wedge
(semi-angle 15◦_{) is pushed in between at constant velocity (38}_{µm/s) up to crack initiation. The SIF}
*K*is observed to decrease with the crack length*c*[40]. In order to increase its value at crack initiation,
and therefore the initial crack velocity, a circular hole with a radius ranging between 2 and 8mm is
drilled at the tip of the groove to tune the stored mechanical energy*U*0, and therefore the range of
*K*(*t*) andv(*t*) scanned over a given experiment. Dynamic crack growth with instantaneous velocities
ranging from 75 m.s−1_{to 500 m.s}−1_{and stable trajectories are obtained. The location}_{c}_{(}_{t}_{) of the crack}
front is measured during each experiment (40µm and 0.1µs accuracies) using a modified version of
the potential drop technique: A series of 90 parallel conductive lines (2.4 nm-thick Cr layer covered
with 23 nm-thick Au layer), 500µm-wide with an*x*-period of 1*mm*are deposited on one of the*x*-y
surfaces of the specimen, connected in parallel and alimented with a voltage source. As the crack
prop-agates, it cuts the conductive lines at successive times that can be detected via an oscilloscope. The
instantaneous crack velocityv(*c*) is computed from*c*(*t*). The value of the stress intensity factor*K*(*c*)
is calculated using 2D finite element calculations (software Castem 2007) on the exact experimental
geometry, assuming plane stress conditions and a constant wedge position as boundary condition. The
calculations have been checked by comparison with the results of a previous finite elements study by
Karihaloo and Xiao [40].

**3 Results**

**3.1 Determination of the fracture energy**

### 0

### 100

### 200

### 300

### 400

### 0

### 0.5

### 1

### 1.5

### 2

### 2.5

### 3

### 3.5

### 4

### Crack velocity (m.s

−1### )

### Fracture energy (kJ.m

−2

### )

### v

_{a}

### v

_{b}

**Fig. 2.**Adapted from [38]. Fracture energyΓas a function of crack velocityvfor five different experiments with

different stored mechanical energies*U*0at crack initiation: 2.0 (), 2.6 (_{◦}), 2.9 (♦), 3.8 (+) and 4.2 J (_{×}). The two

vertical dashed lines correspond tov*a*andv*b*. The two horizontal dashed lines indicate the confidence interval for

the measured fracture energy*K*2

*c*/*E*at crack initiation. Thick line: model prediction (see section 4).

Eq. 1. Its variations as a function ofv, plotted in Fig. 2, is found to be the same in various experiments
performed with various stored mechanical energy *U0* >2.0 J at crack initiation. Three regimes can
be evidenced on this curve. For slow crack velocities,Γremains of the order of*Kc*2/*E*as expected in

LEFM. Then, asvreaches the first critical velocityv*a*≃165 m.s−1=0.19*cR*,Γincreases abruptly to a

value about 3 times larger than*K*2

*c*/*E*. Beyondv*a*,Γincreases slowly withvup to the second critical

velocity, v*b*=0.36*cR* ≃ 317 m.s−1 [10], above which Γdiverges again withv. This second increase
corresponds to the onset of the micro-branching instability, widely discussed in the literature [11]
[10], whereas the first one, atv*a*, was reported in [38] for the first time. The high slope ofΓ(v) around

v*a*provides a direct interpretation for the repeated observation of cracks that span a large range ofΓ

but propagate at a nearly constant velocity of about 0.2*cR*(see e.g. refs. [45] [46]).

**3.2 Morphology of post-mortem fracture surfaces**

To shed light on the nature of the transition atv=v*a*evidenced on the curve relatingΓtov(Fig. 2),

we examine now the post mortem fracture surfaces. Figure 3 shows the evolution of the surfaces
morpholoy as the velocity increases. For vsmaller than v*a*, the fracture surface remains smooth at

the optical scale, as in Fig. 3a (bottom). But above this threshold, conic marks can be evidenced on
the fracture surfaces (Figs. 3b and c, bottom). They do not leave any visible print on the side of the
specimens (Fig. 3a and b, top), contrary to the micro-branches that start to develop at higher velocities,
forv_{≥}v*b*(Fig. 3c, top).

## a

## b

## c

**Fig. 3.**Adapted from [38]. Microscope images (_{×}10) taken at (a)v=120_{±}20 m.s−1_{,}* _{K}*2

_{/}

_{E}_{=1 kJ.m}−2

_{(b)}

_{v}

_{=260}

±30

m.s−1_{,}* _{K}*2

_{/}

_{E}_{=2 kJ.m}−2

_{(c)}

_{v}

_{=650}

_{±}

_{100 m.s}−1

_{(}

*2*

_{K}_{/}

_{E}_{=7 kJ.m}−2

_{). Top line : sample sides (0}

_{.}

_{25}

_{×}

_{0}

_{.}

_{7 mm}2

_{field of}

view). Bottom line : fracture surfaces (0.5×0.7 mm2field of view). Crack propagation is from left to right.

Similar conic marks were reported in the fracture of other brittle materials, among which polystyrene [41], silicate glasses [42], cellulose acetate [43], polycrystalline materials [44], and Homalite [46]. Their formation is thought [42] to find their origin in the heterogeneous nature of the material, which contains inherent toughness fluctuations at the microstructure scale. The enhanced stress field in the vicinity of the main crack front activates some of the low toughness zones and triggers the initiation of secondary penny-shape microcracks ahead of the crack front. These microcracks grow radially under the stress imposed by the main crack along a plane different from that of the main crack. And when these two fronts intersect in space and time, the ligament separating the two cracks breaks up leaving a conic marking on the post-mortem fracture surface.

Figure 4 shows the surface density of conic marksρas a function of crack velocityv. Belowv*a*,

we checked that no conic mark is observable up to_{×}50 magnification. Abovev*a*,ρincreases almost

linearly withv_{−}v*a*. The precise correspondence between the critical velocityv*a*at which the slope of

### 0

### 100

### 200

### 300

### 400

### 0

### 10

### 20

### 30

### 40

### 50

### 60

### 70

### Crack velocity (m.s

−1### )

### Density of conic marks (mm

−

2

### )

### v

_{a}

### v

_{b}

**Fig. 4.**Adapted from [38]. Surface densityρof conic marks as a function of crack velocity for the same
experi-ments as in Fig. 2.

strongly suggests that both phenomena are associated with the same transition. The nucleation, growth
and coalescence of micro-cracks can therefore be identified as the new fracture mechanism starting at
v*a*. This damage process is generic in brittle materials and is relevant for an even wider range of

materials than those that exhibit conic marks, e.g. granite [47].

**4 Interpretation**

We turn now to the interpretation of the curvesΓ(v) between 0 andv*b*. In this respect, it is interesting to

plotΓ(v) as a function of the dynamic SIF*Kd*(v) (Fig. 5(a)). This quantity can be related to the static SIF

*K*through:*Kd*(v)=*k*(v)*K*[4] where*k*(v)≃(1−v/*cR*)/√1−v/*cD*is universal and*cD*is the dilatational

wave speed (here*cD*=2010±60 m.s−1). Below and abovev*a*,Γis found to vary linearly with*Kd*(v)2

(Note thatΓhas been plotted as a function of *Kd*(v)2/*E* rather than*Kd*(v)2 so that both coordinates

are in J/m2_{). This scaling is to compare to that of the size}_{R}

*c*(v) of the Fracture Process Zone (FPZ),

i.e. the zone where linear elasticity fails and all the dissipative phenomena occur:*Rc*(v)= *Kd*2(v)/*a*σ2*Y*

whereσ*Y*is the yield stress and*a*is a dimensionless constant (see e.g. [37]).

Let us first look at the regime before micro-cracking (v ≤v*a*). The affine relation betweenΓand

*Rc*(v) suggests that the volume energyǫ dissipated within the FPZ is constant. Indeed, the volume

scanned by the FPZ when the crack surface increases by*S* is*Rc*(v)*S*. The dissipated energyΓ(v)*S* is

given byγ*S* +ǫ*Rc*(v)*S* whereγis the Griffith surface energy. SinceΓ(v=0)=*Kc*2/*E*, one finally gets

forv_{≤}v*a*:

Γ(v)=α*Kd*(v)
2

*E* +(1−α)
*K*2

*c*

*E* with α=
2ǫ*E*

*a*σ2* _{Y}* (2)

A linear fit to the data (*R*=0.985) givesα=1.17_{±}0.05 and*K _{c}*2/

*E*=0.3

_{±}0.2 kJ.m−2

_{(see Fig. 5(a)).}The latter value is compatible with the measurements of the fracture energy at crack initiation.

By combining Eqs. (1) and (2), one gets a prediction for theΓ(v) curve [48] which reproduces very
well the regime below the micro-cracking onset,v_{≤}v*a*(Fig. 2, thick line). Extrapolation of this regime

exhibits [48] a divergence of the dissipated energy for a finite velocityv′

0 1 2 3 4 5
0
10
20
30
40
50
60
70
*K*
*d*
*2*

*/E (kJ/m2)*

ρ
* (*
*m*
*m*
*−*
*2* *)*
K
a
2
/E

0 1 2 3 4 5

0 0.5 1 1.5 2 2.5 3 3.5 4 K d 2

/E (kJ.m−2)

Frac tu re en er g y ( kJ.m −2 )

K_{a}2/E

Γ_{a}

**Fig. 5.**Adapted from [38]. (a) Dynamic fracture energyΓas a function of*K _{d}*2/

*E*. A crossover between two linear

regimes (linear fits in black lines) occurs at*K*2

*d*/*E* = *K*2*a*/*E* ≃1.2 kJ.m−2,Γ = Γ*a* ≃1.34 kJ.m−2_{). (b) Surface}

density of conic marksρas a function of*K*2

*d*/*E*(linear fit in black line).

200 m.s−1_{≃}_{0.23}_{c}_{R}_{, slightly larger than}_{v}_{a}_{. In the absence of micro-cracks, this velocity}_{v}′

*a*would have

therefore set the limiting macroscopic crack velocity.

Forv≥v*a*, micro-cracks start to nucleate. The existence of a threshold for micro-cracking appears

surprising because it cannot be accounted for by a stress-driven nucleation mechanism only. We believe
that the conic marks observed here correspond to the fraction of micro-cracks that have had sufficient
time to develop up to optical scale. Indeed, when the FPZ is too small (e.g. forv≤v*a*), the nucleated

micro-cracks are rapidly caught up by the main crack, only leaving submicrometric elliptic marks, undetectable with×50 optical microscope.

To interpret the curveΓ(v) within the micro-cracking regime, i.e. forv*a* ≤ v≤ v*b*, we invoke the

existence of an excluded volume*V*around each micro-crack where stresses are screened and therefore
dissipation is prevented. As before, it is interesting to plot the surface density of conic marksρ(v) as
a function of*Kd*(v) (Fig. 5(b)). Note that the limiting velocity for individual crack/micro-crack tips is

expected to bev′

*a*&v*a*. It is then natural to assume that all micro-cracks propagate at the same velocity

v*a*in the microcracking regime, which yields*Kd*(v)=*k*(v*a*)*K*. Between*Ka*= *Kd*(v*a*) and*Kb*=*Kd*(v*b*),

ρ(v) is observed to scale as:

ρ(v)=β*Kd*(v)
2

−*Ka*2

*E* (3)

where a fit to the data (*R*=0.877) givesβ=33±3 J−1. This square dependency indicates that the number

of conic marks is proportional to the FPZ size and suggests that the density of nucleation sites for
micro-cracks is constant within the material. In the micro-cracking regime, the energyΓ(v)*S* dissipated
when the crack surface increases by*S* isγ*S* +ǫ(*Rc*(v)*S* −ρ(v)*S V*), yielding:

Γ(v)=Γ*a*+χ*Kd*(v)

2

−*Ka*2

*E* with χ=α−ǫβ*V* (4)

withΓ*a*the fracture energy obtained atv=v*a*using Eq. 2. Equation (4) predicts a linear dependence

ofΓwith*Kd*(v)2/*E*, which is in agreement with the measurements for*Kd*(v)2/*E* > *Ka*2/*E*(Fig. 5(a)).

A linear fit to the data (*R*=0,948) givesχ=0.67±0.01.

The corresponding predictedΓ(v) [48] reproduces very well the intermediate velocity regimev*a*≤

v≤v*b*(Fig. 2) and exhibits a divergence of the dissipated energy forv∞=*cR*(1−χ*k*(v*a*)2)≃450 m.s−1≃
0.52*cR*. This limiting velocity is very close to the observed maximum crack speed in brittle amorphous

**5 Conclusion**

Both the experimental results and the above discussion shed light on how material defects might
con-trol the dynamic fracture of amorphous solids before the onset of micro-branching. Forv < v*a*, the

mechanical energy released at the crack tip is dissipated into both a constant surfacic energy and a
volumic energy within the FPZ. Since the size of the latter increases rapidly with crack speed, in the
absence of micro-cracks, the fracture energy would diverge at a value slightly larger thanv*a*. At this

point, the crack speed would saturate. In reality, through the nucleation, growth and coalescence of
micro-cracks, the main crack can reach with a larger effective (macroscopic) velocity [46] [49], up to
v*b*=0.4*cR*. The latter value is determined by the onset of micro-branching, that adds to micro-cracking.

We emphasize that the*nominally brittle to quasi-brittle transition*occurring atv*a*should be generic for

amorphous solids and should therefore be taken into account in future conceptual and mathematical descriptions of dynamic fracture. In particular, a better understanding of the relationship between the dynamics of propagation of both the individual micro-cracks and the macroscopic crack is required.

**References**

1. A.A. Griffith, Philosophical Transactions of the Royal Society of London, Series A**221**, (1920) 163
2. E. Orowan, Welding Journal, Research Supplement**34**(1955) 157

3. G.R. Irwin, Handbuch der Physik,**6**, (1958) 551.

4. L. Freund,*Dynamic Fracture Mechanics*(Cambridge University Press, Cambridge, England, 1990)
5. H. Bergkvist, Engineering Fracture Mechanics**6**, (1974) 621

6. J. Fineberg and M. Marder, Physics Reports**313**, (1999) 1

7. K. Ravi-Chandar,*Dynamic Fracture*(Elsevier, Amsterdam, The Netherlands, 2004)
8. A. Livne, O. Ben-David and J. Fineberg, Physical Review Letters**98**, (2007) 124301
9. A. Livne, E. Bouchbinder and J. Fineberg, Physical Review Letters**101**, (2008) 264301
10. E. Sharon and J. Fineberg, Nature**397**, (1999) 333

11. J. Fineberg, S.P. Gross, M. Marder and H.L. Swinney, Physical Review Letters**67**, (1991) 457
12. J. Fineberg, S.P. Gross, M. Marder and H.L. Swinney, Physical Review B**45**, (1992) 5146
13. M. Adda-Bedia, M. Ben Amar and Y. Pomeau, Physical Review E**54**, (1996) 5774
14. P. Gumbsch, S.J. Zhou, B.L. Holian, Physical Review B**55**, (1997) 3445

15. M. Adda-Bedia, R. Adias, M. Ben Amar and F. Lund, Physical Review Letters**82**, (1999) 2314
16. M. Adda-Bedia, Physical Review Letters**93**, (2004) 185502

17. H. Henry and H. Levine, Physical Review Letters**93**, (2004) 105504

18. E. Bouchbinder, J. Mathiesen and I. Procaccia, Physical Review E**71**, (2005) 056118

19. R. Spatschek, M. Hartmann, E. Brener, H. Muller-Krumbhaar and K. Kassner, Physical Review
Letters**96**, (2006) 015502

20. D. Pilipenko, R. Spatschek, E.A. Brener and H. Muller-Krumbhaar, Physical Review Letters**98**,
(2007) 015503

21. E. Katzav, M. Abba-Bedia and A. Arias, International Journal of Fracture,**143**, (2007) 245
22. H. Henry, EPL**83**, (2008) 16004

23. J.F. Kalthoff, S. Winkler and J. Beinert, International Journal of Fracture**71**, (1976) 317

24. A.J. Rosakis, J. Duffy and L.B. Freund, Journal of the Mechanics and Physics of Solids**32**, (1984)
443

25. C. Fond and R. Schirrer, Comptes Rendus de l’Acad´emie des Sciences de Paris*329*, (2001) 195
26. A. Bertram and J.F. Kalthoff, Materialpr¨ufung**45**, (2003) 100

27. D. Hull, *Fractography: Observing, Measuring and Interpreting Fracture Surface Topography*
(Cambridge University Press, Cambridge, England,

33. G. Wang, Y.T. Wang, Y.H. Liu, M.X. Pan, D.Q. Zhao and W.H. Wang, Applied Physics Letters
**89**, (2006) 121909

34. M.J. Buehler and H. Gao, Nature**439**, (2006) 307

35. G. Wang, D.Q. Zhao, H.Y. Bai, M.X. Pan, A.L. Xia, B.S. Han, X.K. Xi, Y. Wu and W.H. Wang,
Physical Review Letters**98**, (2007) 235501

36. A. Rabinovitch and D. Bahat, Physical Review E**78**, (2008) 067102

37. B. Lawn,*Fracture of Brittle Solids*(Cambridge University Press, Cambridge, England, 1993)
38. J. Scheibert, C. Guerra, F. C´elari´e, D. Dalmas and D. Bonamy, Physical Review Letters **104**,

(2010) 045501

39. E. Bruhwiler and F.H. Wittmann, Engineering Fracture Mechanics**35**, (1990) 117
40. B.L. Karihaloo and Q.Z. Xiao, International Journal of Fracture**112**, (2001) 120
41. V. R.Regel, Zhurnal Tekhnicheskoi Fiziki**21**, (1951) 287

42. A. Smekal, Osterreich Ingenieur Archiv**7**, (1953) 49

43. J. A. Kies and G. R. Irwin, Journal of Applied Physics**21**, (1950) 716

44. G. R. Irwin and J. A. Kies, Welding Journal Research Supplement**31**, (1952) 95
45. K. Ravi-Chandar and W.G. Knauss, International Journal of Fracture**26**, (1984) 141

46. K. Ravi-Chandar and B. Yang, Journal of the Mechanics and Physics of Solids**45**, (1997) 535
47. D.E.Moore and D.A. Lockner, Journal of Structural Geology**17**, (1995) 95

48. C. Guerra*et al.*, to be published